Poly(ethylene glycol)-containing hydrogels promote the release of primary granules from human blood-derived polymorphonuclear leukocytes Hannah Caitlin Cohen,1 Tyler Jacob Lieberthal,2 W. John Kao1,2,3 1
Pharmaceutical Sciences Division, School of Pharmacy, University of Wisconsin-Madison, 777 Highland Avenue, Madison, Wisconsin 53705 2 Department of Biomedical Engineering, University of Wisconsin-Madison, 1550 Engineering Drive, Madison, Wisconsin 53706 3 Department of Surgery, School of Medicine and Public Health, University of Wisconsin-Madison, 600 Highland Avenue, Madison, Wisconsin 53792 Received 23 January 2014; accepted 29 January 2014 Published online 00 Month 2014 in Wiley Online Library (wileyonlinelibrary.com). DOI: 10.1002/jbm.a.35101 Abstract: Polymorphonuclear leukocytes (PMNs) are recruited to sites of injury and biomaterial implants. Once activated, PMNs can exocytose their granule subsets to recruit monocytes (MCs) and mediate MC/macrophage activation. We investigated the release of myeloperoxidase (MPO), a primary granule marker, and matrix metalloproteinase-9 (MMP-9), a tertiary granule marker, from human blood-derived PMNs cultured on poly(ethylene glycol) (PEG) hydrogels, polydimethylsiloxane (PDMS), tissue culture polystyrene (TCPS) and gelatin–PEG (GP) hydrogels, with and without the presence of the bacterial peptide formyl-Met-Leu-Phe. Supernatants from PMN cultures on PEG-containing hydrogels (i.e., PEG and GP hydrogels) had higher concentrations of MPO than those from PMN cultures on PDMS or TCPS at 2 h. PMNs on all biomaterials released comparable levels of MMP-9 at 2 h, indicating
that PMNs cultured on PEG-containing hydrogels have different mechanisms of release for primary and tertiary granules. Src family kinases were involved in the release of MPO from PMNs cultured on PEG hydrogels, TCPS and GP hydrogels and in the release of MMP-9 from PMNs cultured on all four biomaterials. The increased release of primary granules from PMNs on PEG-containing hydrogels did not significantly increase MC chemotaxis, indicating that additional co-effectors in the dynamic inflammatory milieu in vivo modulate PMNC 2014 Wiley Periodicals, Inc. J Biomed mediated MC recruitment. V Mater Res Part A: 00A:000–000, 2014.
Key Words: Neutrophil, acute inflammation, degranulation, myeloperoxidase, matrix metalloproteinase-9, poly(ethylene glycol)
How to cite this article: Cohen HC, Lieberthal TJ, Kao WJ. 2014. Poly(ethylene glycol)-containing hydrogels promote the release of primary granules from human blood-derived polymorphonuclear leukocytes. J Biomed Mater Res Part A 2014:00A:000–000.
Implantation of a biomaterial initiates a series of inﬂammatory and wound healing events collectively termed the foreign body response (FBR), during which polymorphonuclear leukocytes (PMNs; neutrophils) extravasate to the implant site in response to injury to vascular tissue.1,2 PMNs contain four subsets of granule proteins, formed sequentially based on the biosynthetic capabilities of the cell at the given stage of myelopoeisis (Supporting Information Fig. 1).3 These subsets include primary granules, secondary granules, tertiary granules and secretory vesicles.4 There are nearly 300 granule proteins, including antimicrobial proteins, proteases, b2-integrin receptors, chemotactic receptors and soluble mediators of inﬂammation.5,6 Upon receptor-mediated activation, PMNs can release their granule
subsets to facilitate monocyte (MC) chemotaxis and mediate MC/macrophage activation and function,7–18 thereby inﬂuencing subsequent inﬂammatory or wound healing events in the FBR. To better understand how biomaterials modulate PMN-MC paracrine interactions, in a previous study, we cultured human blood-derived MCs on poly(ethylene glycol) (PEG) hydrogels, polydimethylsiloxane (PDMS) and tissue culture polystyrene (TCPS) and primed the MCs for 24 h with conditioned media from cultures of autologous PMNs pre-activated with matching biomaterials (PMN-conditioned media; PCM).19 PCM signiﬁcantly increased MC viability/adhesion on PEG hydrogels.19 We hypothesized that biomaterial-dependent PMN degranulation may contribute to the observed increase in MC viability/ adhesion upon treatment with PCM from PMN cultures on
Additional Supporting Information may be found in the online version of this article. Correspondence to: W. John Kao; e-mail: [email protected]
Contract grant sponsor: Department of Defense through a National Defense Science and Engineering Graduate fellowship (to H.C.); contract grant number: NIH HL115482
C 2014 WILEY PERIODICALS, INC. V
PEG hydrogels. Therefore, in this study, we sought to determine how biomaterials inﬂuence PMN degranulation events, as PMN granule proteins have implications for downstream inﬂammatory response. We focused on the release of primary and tertiary granules to investigate both early and late degranulation events. PMN primary granules contain toxic antimicrobial reagents such as myeloperoxidase (MPO), human neutrophil peptides 1–3 (HNP1–3), cathepsin G and elastase, and are generally released only after PMN extravasation to the site of inﬂammation.16 PMN tertiary granules contain matrixdegrading enzymes such as matrix metalloproteinase-9 (MMP9) and are released when PMNs transmigrate through the endothelium on their journey to the site of inﬂammation.16 Proteases such as elastase, cathepsin G, and MMP-9 are involved in tissue remodeling in inﬂammation but are also involved in tissue pathology in inﬂammatory diseases.20–22 In addition to the biomaterials we used in our previous study (PEG hydrogels, PDMS and TCPS),19 we also investigated gelatin–PEG (GP) hydrogels, which are a hybrid biomatrix developed in our group based on the thiol-ene reaction of PEG diacrylate and cysteine/PEG-modiﬁed gelatin.23 The incorporation of gelatin in the hydrogel introduces cell-binding motifs such as RGD (arginine-glycine-aspartic acid) peptides and could possibly regulate MMP expression.
MATERIALS AND METHODS
PEG hydrogel, GP hydrogel, PDMS, and TCPS preparation PEG diacrylate (molecular weight 3350) and cysteine/PEGmodiﬁed gelatin (gel-PEG-cys) were synthesized as previously described23 and characterized by proton NMR (Varian UnityInova 400 MHz; Varian Inc., Palo Alto, CA). The proton NMR spectrum of PEG diacrylate in deuterated chloroform showed peaks at 3.6, 3.7, and 4.3 ppm (methylene protons), and 5.8, 6.2, and 6.4 ppm (acrylate protons). PEG diacrylate products were routinely found to have > 85% acrylation based on proton NMR peak area measurements. The proton NMR spectrum of gel-PEG-cys in deuterated water showed peaks at 1.3 ppm (d, 2H, -CH2SH), 2.9 ppm (t, 1H, ACHCH2SH), 3.7 ppm (m, ACH2A from PEG backbone) and broad gelatin peaks at 1.7, 1.8, 1.9, 3.2, and 4.2 ppm. PEG hydrogels were prepared by dissolving 10 wt % PEG diacrylate (molecular weight 3350) and 0.1 wt % 2-hydroxy-4’-(2-hydroxyethoxy)22-methylpropiophenone (Sigma-Aldrich, St. Louis, MO) in water with heat (37 C). GP hydrogels were prepared by dissolving 10 wt % PEG diacrylate (molecular weight 3350), 0.1 wt % 2-hydroxy4’-(2-hydroxyethoxy)22-methylpropiophenone and 10 wt % gel-PEG-cys in water with heat (37 C). The PEG and GP hydrogel solutions were injected into Teﬂon molds held between two, pre-cleaned glass slides and polymerized by placing the assemblies under a UV light (UV CF1000 LED, kmax 5 365 nm; Clearstone Technologies, Minneapolis, MN) for 3 min per side. The PEG and GP hydrogel ﬁlms were cold sterilized in 70% ethanol (Decon Labs, King of Prussia, PA) for 45 min and equilibrated overnight in Dulbecco’s phosphate-buffered saline (DPBS; Cellgro, Manassas, VA). The PEG and GP hydrogel ﬁlms were cut into 8-mm diameter disks with biopsy punches (Mil-
COHEN ET AL.
tex, York, PA), placed into 48-well culture plates (Corning, Corning, NY) and cold sterilized in 70% ethanol for 45 min. PDMS (0.762-mm thickness, non-reinforced vulcanized gloss/gloss; Specialty Manufacturing Inc., Saginaw, MI) was cut into 8-mm diameter disks with biopsy punches and sonicated for 10 min in a 0.5 wt % solution of sodium dodecyl sulfate (Amresco, Solon, OH). The PDMS disks were rinsed with deionized water, placed into 48-well culture plates and cold sterilized in 70% ethanol for 45 min. Sterilized PEG hydrogels, GP hydrogels and PDMS disks were washed three times with DPBS and equilibrated in RPMI-1640 basal medium (Cellgro, Manassas, VA) before seeding with cells. TCPS wells (Corning, Corning, NY) were also washed three times with DPBS and equilibrated in RPMI-1640 medium before cell seeding. Culture of human blood-derived PMNs and MCs Peripheral whole blood was obtained from consenting healthy adult donors in accordance with protocols approved by the University of Wisconsin-Madison Institutional Review Board. PMNs and MCs were isolated as previously described using a gradient method.24 A small percentage (